**Conductance enhancement in quantum-point-contact semiconductor-superconductor devices**

Niels Asger Mortensen and Antti-Pekka Jauho

*Mikroelektronik Centret, Technical University of Denmark, Ørsteds Plads, Building 345 East, DK-2800 Kgs. Lyngby, Denmark*

Karsten Flensberg

*O*”*rsted Laboratory, Niels Bohr Institute, University of Copenhagen, Universitetsparken 5, DK-2100 Copenhagen Ø, Denmark*

Henning Schomerus

*Instituut–Lorentz, Universiteit Leiden, P.O. Box 9506, 2300 RA Leiden, The Netherlands*

共Received 12 March 1999兲

We present numerical calculations of the conductance of an interface between a phase-coherent
two-dimensional electron gas and a superconductor with a quantum point contact in the normal region. Using a
scattering matrix approach we reconsider the geometry of De Raedt, Michielsen, and Klapwijk关Phys. Rev. B
**50, 631**共1994兲兴which was studied within the time-dependent Bogoliubov–de Gennes formalism. We find that
*the factor-of-2 enhancement of the conductance GNScompared to the normal state conductance GN*for ideal
interfaces may be suppressed for interfaces with a quantum point contact with only a few propagating modes.
The suppression is found to depend strongly on the position of the Fermi level. We also study the suppression
due to a barrier at the interface and find an anomalous behavior caused by quasiparticle interference. Finally,
we consider the limit of sequential tunneling and find a suppression of the factor-of-2 enhancement which may
explain the absence of conductance enhancement in experiments on metal-superconductor structures.
关S0163-1829共99兲07943-6兴

**I. INTRODUCTION**

Charge transport through a normal-conductor– superconductor 共NS兲 interface is accompanied by a conver-sion of quasiparticle current to a supercurrent. In the An-dreev reflection, by which the conversion occurs, an electronlike quasiparticle in the normal conductor 共with an excitation energy lower than the energy gap of the supercon-ductor兲incident on the NS interface is retroreflected into a holelike quasiparticle共with reversal of its momentum and its energy relative to the Fermi level兲and a Cooper pair is added to the condensate of the superconductor.1 For an ideal NS interface, the signature of Cooper pair transport and the An-dreev scattering is a doubling of the conductance compared to the normal state conductance.

A theoretical framework for studies of the scattering at NS interfaces is provided by the Bogoliubov–de Gennes 共BdG兲formalism,2where the scattering states are eigenfunc-tions of the BdG equation

### 冉

*Hˆ*

_{共}

_{r}_{兲}⌬共

**r**兲

⌬*共**r**兲 ⫺*Hˆ*_{*}_{共}_{r}_{兲}

### 冊

### 冉

*u*共

**r**兲

*v*共**r**兲

### 冊

⫽*E*

### 冉

*u*共**r**兲

*v*共**r**兲

### 冊

, 共1兲which is a Schro¨dinger-like equation in electron-hole space
共Nambu space兲. Here *H ˆ (r) is the single-particle *
Hamil-tonian,⌬

**(r) is the pairing potential of the superconductor, E**

**is the excitation energy, and u(r) and***v*

**(r) are wave**func-tions of electronlike and holelike quasiparticles.

The technological possibility of studying the interface be-tween a two-dimensional electron gas共2DEG兲in a semicon-ductor heterostructure and a superconsemicon-ductor experimentally, has provided a playground for investigating the interplay

be-tween the Andreev reflection and the mesoscopic effects seen in mesoscopic semiconductor structures.3,4 In recent years the technological efforts have revealed a variety of new me-soscopic phenomena, see Refs. 4–7, and references therein. One class of the studied devices are the quantum point con-tact共QPC兲2DEG-S and S-2DEG-S devices with the QPC in the normal region. The dc Josephson effect and the quanti-zation of the critical current in QPC S-2DEG-S junctions have been studied extensively both experimentally by, e.g., Takayanagi and co-workers8 and theoretically by, e.g., Beenakker and van Houten,9,10 Beenakker,11 and Furusaki, Takayanagi, and Tsukada.12

The linear-response conducting properties of QPC
2DEG-S structures have been studied by several groups. In
the analytical work of Beenakker13a ballistic normal region
with a QPC modeled by a saddle-point potential was
consid-ered. The effect of elastic impurity scattering was considered
numerically by Takagaki and Takayanagi14who considered a
disordered region between a narrow-wide共NW兲constriction
and the superconductor. Both of these studies of the
*conduc-tance were based on a scattering matrix (S-matrix*兲approach
and the BdG formalism. In the numerical simulations of De
Raedt, Michielsen, and Klapwijk,15 based on the
time-dependent BdG equation, a wide-narrow-wide 共WNW兲
con-striction was considered. Here, the aim was to study the
electron-hole conversion efficiency and the robustness of the
back-focusing phenomena of the Andreev reflection.

One of the properties of the QPC is that most transmission eigenvalues are either close to zero or unity. For an ideal QPC 2DEG-S interface, the Andreev reflection will therefore give rise to a factor-of-2 enhancement of the conductance

*G*NS *compared to the normal state conductance G*N,10,13
*which is quantized in units of 2e*2*/h.*16However, as pointed

PRB 60

out by van Houten and Beenakker,10 deviations from the simple factor-of-2 enhancement should be expected when the position of the Fermi level does not correspond to a conduc-tance plateau. The presence of impurity scattering in the nor-mal region and/or interface roughness will also suppress the doubling of the conductance.14

*Using an S-matrix approach, we study the linear-response*
regime of a phase-coherent ballistic QPC 2DEG-S system
where the QPC is modeled by a WNW constrictions with a
hard-wall confining potential, see Fig. 1. We report new
*re-sults for the device studied by De Raedt et al.*15which had a
*relative width W/W*

### ⬘

⫽1.7 m/(1.6⫻335 Å)⯝31.72, an*aspect ratio L*1

*/W*

### ⬘

⫽*5/1.6, and a relative length L*2

*/W*

### ⬘

⫽*20/1.6. Applying the S-matrix formalism instead of the*
computationally more complicated time-dependent BdG
for-malism, we are able to study a larger part of the parameter
space where we also consider a barrier 共with a normalized
*barrier strength Z) at the NS interface. We focus on the*
regime with only a few propagating modes in the QPC. In
this regime the transmission eigenvalues of the QPC depend
strongly on the actual position of the Fermi level. Even for
an ideal interface this gives rise to a strong suppression of
the conductance for certain positions of the Fermi level as
predicted by van Houten and Beenakker10 and subsequently
seen in the work of Beenakker.13In the presence of a barrier
at the interface, the QPC gives rise to an enhanced tunneling
through the barrier共compared to the case without a QPC兲as
in the case of reflectionless tunneling effect of diffusive
junctions.13,17

In the sequential tunneling limit the conductance can be
found by considering the QPC and the interface as two
*series-connected resistive regions and in the limit W*Ⰷ*W*

### ⬘

the enhancement of the conductance compared to the normal
state conductance vanishes even for ideal NS interfaces. This
may be an explanation for the unexpectedly low conductance
*enhancement in the experimental results of Benistant et al.*18
on Ag-Pb interfaces where the current is injected into the Ag
crystal through a point contact.

*The text is organized as follows. In Sec. II the S-matrix*
formalism is introduced, in Sec. III we formulate our model,
in Sec. IV the scattering scheme of the considered geometry
is presented, and in Sec. V we present results of several
applications of our scattering scheme. Finally, in Sec. VI
discussion and conclusions are given.

**II. SCATTERING MATRIX FORMALISM**

The scattering approach to coherent dc transport in super-conducting hybrids follows closely the scattering theory de-veloped for nonsuperconducting mesoscopic structures, see, e.g., the text-book by Datta.19For an ideal NS interface, the interface acts as a phase-conjugating mirror within the An-dreev approximation1 and the rigid boundary condition for the pairing potential

⌬共**r**兲⫽⌬0*ei*⌰共*x*⫺*L*兲, 共2兲
where ⌬0 is the BCS energy gap,20 is the phase of the
pairing potential, ⌰*(x) is a Heaviside function, and L*⫽*L*1

⫹*L*2 is the length of the normal region共see Fig. 1兲.
In the linear-response regime in zero magnetic field,
Beenakker13 *found that the conductance G*⬅*I/**V is given*

by

*G*NS⫽
*4e*2

*h* Tr共*tt*

†_{关}_{21ˆ}_{⫺}* _{tt}*†

_{兴}⫺1

_{兲}2

⫽*4e*

2

*h* *n*

### 兺

⫽1*N*

*T _{n}*2

共2⫺*Tn兲*2, 共3兲

which, in contrast to the Landauer formula,21

*G*_{N}⫽*2e*

2

*h* *Tr tt*

†_{⫽}*2e*
2

*h* *n*

### 兺

⫽1*N*

*T _{n}*, 共4兲

*is a nonlinear function of the transmission eigenvalues Tn*
*(n*⫽*1,2, . . . ,N) of tt*†*. Here t is the N*⫻*N transmission *

*ma-trix of the normal region, N being the number of propagating*
modes.

Equation共3兲holds for an arbitrary disorder potential and is a multichannel generalization of a conductance formula first obtained by Blonder, Tinkham, and Klapwijk22 who considered a delta function potential as a model for the in-terface barrier potential. The computational advantage of Eq. 共3兲 over the time-dependent BdG approach of De Raedt

*et al.*15is that we only need to consider the time-independent
Schro¨dinger equation with a potential which describes the
disorder in the normal region, so that we can use the
tech-niques developed for quantum transport in normal
conduct-ing mesoscopic structures. For more details on, e.g., finite
bias and/or temperature, see Lesovik, Fauche`re, and
Blatter,23 Lesovik and Blatter,24 and the reviews of
Beenakker,6and Lambert and Raimondi.7

**III. MODEL**

We describe the geometry of Fig. 1 by the Hamiltonian

*Hˆ*_{共}_{r}_{兲}_{⫽⫺} ប

2

*2m*“*ˆ*⫹*V*␦共**r**兲⫹*V*c共**r**兲⫺, 共5兲
where is the chemical potential. The barrier potential is
*given by a Dirac delta function potential with strength H:*22

*V*_{␦}共**r**兲⫽*H*␦共*x*⫺*L*兲, 共6兲
and the transverse motion is limited by a hard-wall confining
potential

*V*c共**r**兲⫽

### 再

0, 兩*y*兩⬍*W*共*x*兲/2,

⬁, 兩*y*兩⭓*W*共*x*兲/2, 共7兲
where the width*W(x) defines the WNW constriction and is*
given by

*W*共*x*兲⫽

### 再

*W,* *x*⬍0,

*W*

### ⬘

, 0⭐*x*⭐

*L*1,

*W,* *x*⬎*L*1.

共8兲

The scattering states can be constructed as linear combina-tions of the eigenstates of the Schro¨dinger equation.

**IV. SCATTERING SCHEME**

*In the following subsections, we consider the S-matrices*
of a system with the Hamiltonian in Eq.共5兲relevant for the
*geometry shown in Fig. 1. The S-matrix S of a scattering*
*region relates the incident current amplitudes a*_{S}⫾ to the
*out-going current amplitudes b*S⫾. For a scattering region with
*two leads, S is a 2*⫻2 block-matrix with submatrices

*S*11*,S*12*,S*21*, and S*22, where the diagonal and off-diagonal
submatrices are reflection and transmission matrices,
respec-tively. The appropriate scattering scheme for three scattering
regions共the WN and the NW constrictions, and the interface
barrier potential, respectively兲connected by ballistic
conduc-tors is shown in Fig. 2.

*The WN constriction is described by the S-matrix S*WN

### 冉

*b*S⫹

_{1}

*b*_{S}

1

⫺

### 冊

⫽*S*WN

### 冉

*a*S⫹_{1}

*a*_{S}

1

⫺

### 冊

, 共9兲*the narrow region of length L*1*by the propagation-matrix U*N

### 冉

*a*

_{S}

1

⫺

*a*_{S}

2

⫹

### 冊

⫽*U*N

### 冉

*b*_{S}

1

⫺

*b*_{S}

2

⫹

### 冊

, 共10兲*the NW constriction by the S-matrix S*NW

### 冉

*b*

_{S}

2

⫹

*b*_{S}

2

⫺

### 冊

⫽*S*NW

### 冉

*a*_{S}

2

⫹

*a*_{S}

2

⫺

### 冊

, 共11兲*the wide region of length L*2 *by the propagation-matrix U*W

### 冉

*a*

_{S}

2

⫺

*a*_{S}

3

⫹

### 冊

⫽*U*W

### 冉

*b*_{S}

2

⫺

*b*_{S}

3

⫹

### 冊

, 共12兲*and the delta function barrier by the S-matrix S*␦

### 冉

*b*

_{S}

3

⫹

*b*_{S}

3

⫺

### 冊

⫽*S*␦

### 冉

*a*_{S}

3

⫹

*a*_{S}

3

⫺

### 冊

. 共13兲To apply Eqs.共3兲and共4兲 we need to calculate the
*com-posite transmission matrix t*⫽*S*21which is a submatrix of the
*composite S-matrix S*⬅*S*WN丢*U*N丢*S*NW丢*U*W丢*S*␦ relating
the outgoing current amplitudes to the incoming current
am-plitudes

### 冉

*b*S⫹

_{1}

*b*_{S}

3

⫺

### 冊

⫽*S*

### 冉

*a*S⫺_{3}

*a*_{S}

1

⫹

### 冊

*S*⫽

### 冉

*r* *t*

### ⬘

*t* *r*

### ⬘

### 冊

. 共14兲The meaning of the symbol 丢 is found by eliminating the internal current amplitudes.19 As a final result we find the transmission matrix

*t*⫽*S*_{21}␦关*1ˆ*⫺*U*_{21}W兵*S*NW_{22} ⫹*S*_{21}NW关*1ˆ*⫺*U*_{21}N*S*_{22}WN*U*_{12}N*S*_{11}NW兴⫺1*U*_{21}N*S*_{22}WN*U*_{12}N*S*_{12}NW其*U*_{12}W*S*_{11}␦兴⫺1

⫻*U*_{21}W*S*_{21}NW关*1ˆ*⫺*U*_{21}N*S*_{22}WN*U*_{12}N*S*_{11}NW兴⫺1*U*_{21}N*S*_{21}WN. 共15兲

**A. Quantum point contact**

We consider a QPC which we model by a WNW constric-tion defined by a hard-wall confining potential, see Fig. 1. This geometry has been considered by Szafer and Stone25 and Weisshaar, Lary, Goodnick, and Tripathi26in the context of conductance quantization of the QPC in a 2DEG, and recently by Kassubek, Stafford, and Grabert27in the context of conducting and mechanical properties of ideal two and three-dimensional metallic nanowires. We follow Kassubek

*et al.*27 *and calculate the composite S-matrix S*WNW_{⫽}* _{S}*WN

丢*U*N丢*S*NW*. In zero magnetic field, where all S-matrices *
*sat-isfy S*⫽*ST, the individual S-matrices are given by*

*S*WN⫽

### 冉

*r*_{NW}

### ⬘

*t*NW

*t*_{NW}*T* *r*_{NW}

### 冊

, 共16兲*U*N⫽

### 冉

*0ˆ* *X*N

*X*N

*0ˆ*

### 冊

, 共17兲*S*NW⫽

### 冉

*r*NW *t*NW
*T*

*t*_{NW} *r*_{NW}

### ⬘

### 冊

, 共18兲*where X _{nn}*
⬘

N _{⫽}_{␦}

*nn*⬘*exp (iknL*1) describes the narrow region
with free propagation of propagating modes and an
exponen-FIG. 2. Scattering scheme appropriate for the normal region of

tial decay of evanescent modes. Here *kn*

⫽*k*F冑1⫺*(n**/k*F*W*

### ⬘

)2 is the longitudinal wave vector of*mode n in the narrow region. The S-matrices of the WN and*NW constrictions are related through an exchange of leads.

By elimination of the internal current amplitudes we find the composite transmission matrix

*S*WNW⫽

### 冉

*r*WNW *t*WNW

*t*WNW *r*WNW

### 冊

, 共19兲

where

*r*WNW⫽*r*NW

### ⬘

⫹*t*NW关

*1ˆ*⫺共

*X*N

*r*NW兲2兴⫺1

*X*N

*r*NW

*X*N

*t*NW

*T*

, 共20兲

*t*WNW⫽*t*NW关*1ˆ*⫺共*X*N*r*NW兲2兴⫺1*X*N*t*NW
*T*

. 共21兲

*The S matrix of the NW constriction can be found from a*
matching of scattering states which are eigenstates of the
Schro¨dinger equation with the Hamiltonian in Eq.共5兲where
we only consider the part of the potential which sets up the
NW constriction. From a matching of scattering states we
find that

*r*NW⫽共*1ˆ*⫹*%%T*兲⫺1共*1ˆ*⫺*%%T*兲, 共22兲

*t*NW⫽2*%T*共*1ˆ*⫹*%%T*兲⫺1, 共23兲

*r*_{NW}

### ⬘

⫽共*%T%*⫹

*1ˆ*兲⫺1共

*%T%*⫺

*1ˆ*兲, 共24兲 where the elements of the

*%*matrix can be written as

*%*

_{nw}⫽

### 冑

*Kw/kn*

### 具

*n兩⌽w*

### 典

, where### 具

*n兩⌽w*

### 典

⫽兰_{⫺⬁}⬁

*dy*

*n( y )*⌽w

*( y )*

*is an overlap between transverse wave functions of mode n*

*in the narrow region and mode w in the wide region. Here*

*Kw*⫽*k*F冑1⫺*(w*/*k*F*W*

### ⬘

)2 is the longitudinal wave vector*of mode w in the wide region and*⬅

*W/W*

### ⬘

is the relative width of the constriction.The overlap can be calculated analytically since its
ele-ments consist of overlaps between transverse wave functions
*n*and⌽wwhich are either two sine or two cosine functions
共the overlap between a sine function and a cosine function or
vice versa is zero due to the odd and even character of the
two functions兲. From the overlap-matrix we get the
follow-ing elements of the*%* matrix:

*%nw*⫽␦_{P}(n),_{P}(w)

### 冉

共*k*F*W*

### ⬘

/兲2⫺共*n/*兲2 共

*k*F

*W*

### ⬘

/兲2⫺*n*2

### 冊

1/4

⫻

## 冦

␦*P(n),1*共⫺1兲*(n*⫹2)/2⫻

*4n*3/2sin共*w*/2兲

共*n*22⫺*w*2兲 , *n*⫽*w,*

␦*P(n),*⫺1共⫺1兲*(n*⫺1)/2⫻

*4n*3/2cos共*w*/2兲

共*n*22⫺*w*2兲 , *n*⫽*w,*

⫺1/2_{,} _{n}_{}_{⫽}_{w,}

共25兲

where the parity *P( j ) of j is* *P( j )*⬅*1 if j is even andP( j)*
⬅⫺*1 if j is odd.*

In the numerical evaluation of Eqs. 共22兲–共24兲 and Eqs. 共20兲and共21兲it is crucial to let the number of modes in the narrow and wide regions extend over both propagating modes and evanescent modes. After all matrix inversions are performed, the reflection and transmission matrices are pro-jected onto the propagating modes. In practice, numerical convergence of the reflection and transmission matrices is found for a finite cutoff in the number of evanescent modes. For the considered device, the number of evanescent modes is roughly ten times the number of propagating modes in the wide region corresponding to 1000⫻1000 matrices.

*In the limit W*Ⰷ*W*

### ⬘

, Szafer and Stone25 employed a mean-field approximation for the overlap### 具

*n兩⌽w*

### 典

in which*mode n of the narrow region couples uniformly to only a*band of modes共

*with the same parity as mode n) in the wide*region within one level spacing so that the elements of the

*%*matrix take the form

*%nw⬇*␦*P(n),P(w)*

### 冉

共*k*F*W*

### ⬘

/兲2⫺共*n/*兲2 共

*k*F

*W*

### ⬘

/兲2⫺*n*2

### 冊

1/4

⫻

### 再

⫺1/2_{,} _{共}_{n}_{⫺}_{1}_{兲}_{}_{⭐}_{w}_{⬍}_{共}_{n}_{⫹}_{1}_{兲}_{}_{,}

0, otherwise. 共26兲

*Within this approximation, there is no mode mixing and tt*†
becomes diagonal with the transmission eigenvalues along
the diagonal. This approximation was found to capture the
results of an exact numerical calculation25 when used with
the Landauer formula, Eq. 共4兲, which is linear in the
*trans-mission eigenvalues T _{n}*. However, for an NS interface, the
conductance formula, Eq.共3兲

*, is nonlinear in Tn*which also

*makes off-diagonal components in tt*†important. As we shall see 共in Fig. 3兲, the mean-field approximation cannot

*repro-duce the results of an exact numerical calculation of G*NSin

*the same nice way as for G*

_{N}.

**B. Wide region**

*The wide region L*1⬍*x*⬍*L is described similarly to the*
narrow region by

*U*W⫽

### 冉

*0ˆ* *X*W

*X*W *0ˆ*

### 冊

, 共27兲**C. Interface barrier potential**

*We consider an NS interface of width W with a barrier*
which we model by a Dirac delta function potential,
follow-ing Blonder, Tinkham, and Klapwijk.22 *The S-matrix *
ele-ments for the delta-function potential is found from a
match-ing of scattermatch-ing states which are eigenstates of the
Schro¨dinger equation with the Hamiltonian in Eq.共5兲where
we only consider the part of the potential consisting of the
barrier at the interface. In zero magnetic field one finds the
symmetric result

*S*␦⫽

### 冉

*r*

_{␦}

*t*

_{␦}

*t*_{␦} *r*_{␦}

### 冊

, 共28兲with

共*t*_{␦}兲ww_{⬘}⫽␦*ww*⬘
1

1⫹*iZ/cos**w*

, 共29兲

共*r*_{␦}兲ww_{⬘}⫽␦*ww*⬘

⫺*iZ/cos**w*
1⫹*iZ/cos**w*

, 共30兲

*where the normalized barrier strength is given by Z*
⬅*H/*ប*v*Fand cos*w⬅Kw/k*F⫽

### 冑

1⫺*(w*

*/k*F

*W)*2. The results differ from those of a one-dimensional calculation22since we have taken the parallel degree of freedom into account. How-ever, if we introduce an angle dependent effective barrier

*strength Z*eff(

*w*)⫽

*Z/cos*

*w*,28,29the transmission and reflec-tion amplitudes can formally be written in the one-dimensional form of Ref. 22. The transmission eigenvalues

*of t*

_{␦}

*t*

_{␦}†

*are given by T*␦⫽关1⫹

_{w}*Z*

_{eff}2 (

*w*)兴⫺1 in contrast to the mode-independent result

*T*␦⫽(1⫹

_{w}*Z*2

_{)}⫺1

_{of}

_{a}

_{}one-dimensional calculation.22

**V. RESULTS**

**A. Phase-coherent junction with ideal interface**

For the case of coherent transport through an ideal
2DEG-S interface with a WNW constriction in the normal
*region, see lower inset of Fig. 3, the conductance G*NS and
*the normal state conductance G*Ncan be found from Eqs.共3兲
and共4兲*with the transmission matrix t*⫽*t*WNW. Fig. 3 shows
*the conductance as a function of k*F*W*

### ⬘

/based on a*numeri-cal numeri-calculation of t*

_{WNW}共full lines兲 and the mean-field ap-proximation 共dashed line兲 for a WNW constriction with an

*aspect ratio L*1

*/W*

### ⬘

⫽*1 and a relative width W/W*

### ⬘

⫽31.72.*The conductance G*NSis seen to be approximately quantized

*in units of 4e*2

*/h which is twice the unit of conductance for*

*the normal state conductance G*N. However, just above the

*thresholds (k*

_{F}

*W*

### ⬘

/⫽1,2,3, . . . ), oscillations due to reso-nances in the narrow region of the constriction are observed. In the normal state result, these resonances are small but in*contrast to the Landauer formula, G*NS is not linear in the transmission eigenvalues and this makes the resonances much more pronounced compared to those in the normal state conductance. Another signature of the nonlinearity of

*G*NS and the importance of off-diagonal transmission, is that
the mean-field approximation is in good agreement with the
*numerical calculation for G*N whereas it has difficulties in
*accounting for G*NS. The sharpness of the resonances is to a
certain extent due to the wide-narrow-wide constriction, and
is suppressed in experiments with split-gate-defined
constric-tions. However, as shown by the simulations of Maaø,
Zo-zulenko, and Hauge30 resonance effects do persist even for
more smooth connections of the narrow region to the 2DEG
reservoirs.

*The normalized conductance g*⬅*G*NS*/G*N, shown in the
upper insert, is two on the conductance plateaus but for
cer-tain ‘‘mode fillings’’ of the constriction it is strongly
*sup-pressed and for k*F*W*

### ⬘

/⬃2共two propagating modes兲we get*g*⬃1.5. This effect, which occurs at the onset of new modes,
was also seen in the calculations of Beenakker.13 As the
number of modes increases, these dips vanish and the
nor-malized conductance approaches its ideal value of 2. The
*reason is simple: suppose the constriction has N propagating*
*modes, then the N*⫺1 of them will have a transmission of
order unity and only a single mode 共corresponding to the
mode with the highest transverse energy兲will have
*transmis-sion different from unity. As N increases, the effect of the*
single mode with transmission different from unity becomes
negligible for the normalized conductance and from Eqs.共3兲
and共4兲it follows that lim

*N→*⬁*g*⫽2.

Since the quasiparticle propagation is coherent and the
Andreev scattering is the only back-scattering mechanism,
the phase conjugation between electronlike and holelike
*qua-siparticles makes the conductance G*NS independent of the
*separation L*2of the constriction and the interface. If
evanes-cent modes in this region were also taken into account the
*results would depend weakly on L*_{2} as it was found in the
*simulations of De Raedt et al.*15 and our results should be
*compared with their results in the large L*2 limit. As we shall
see below, interfaces with a finite barrier 共and thereby
*nor-FIG. 3. Conductance GNSand normal state conductance GN*of a

*coherent WNW 2DEG-S junction as a function of k*F*W*⬘/. The
*constriction has an aspect ratio L*1*/W*⬘⫽1 and a relative width

*W/W*⬘⫽31.72. The full lines are for a numerical calculation of

mal scattering at the interface兲lead to size quantization and
*thereby resonances which will depend on L*2.

The back-focusing phenomenon of the Andreev reflected
quasiparticles and the lowering of the normalized
conduc-tance due to a QPC in the normal region was studied by De
Raedt, Michielsen, and Klapwijk15 by solving the
time-dependent BdG equation fully numerically. In their wave
propagation simulations, the QPC is also modeled by a
WNW constriction with a relative width *W/W*

### ⬘

⫽1.7 m/(1.6⫻335 Å)⯝*31.72, an aspect ratio L*1*/W*

### ⬘

⫽*5/1.6, and a relative length L*2*/W*

### ⬘

⫽20/1.6. For the*par-ticular ‘‘mode filling’’ k*F

*W*

### ⬘

/⫽3.2, they find a normalized*conductance g*⫽1.87⬍2, but the dependence on the ‘‘mode filling’’ was not studied in detail.

*In Fig. 4 we present a calculation of g as a function of*

*k*_{F}*W*

### ⬘

/ for this specific geometry. The result of De Raedt*et al. (*䊊) is reproduced but in general the normalized
con-ductance is seen to have many resonances caused by the high
aspect ratio of the constriction. In the range 3⬍*k*F*W*

### ⬘

/⬍4, the normalized conductance can be anything in the
range 1.655⬍*g*⭐2 depending on the position of the Fermi
*level and though De Raedt et al.*15 found the back-focusing
phenomena of the Andreev reflection to be very robust with
respect to changes of the device parameters, the normalized
conductance itself certainly depends strongly on the position
of the Fermi level. The reason is that only those
quasiparti-cles which enter the region between the constriction and the
interface can be Andreev reflected and thus contribute to the
conductance enhancement compared to the normal state
con-ductance.

**B. Phase-coherent junction with barrier at interface**
We next consider coherent transport through an NS
inter-face with a barrier at the interinter-face and a WNW constriction
*at a distance L*_{2} from the interface, see lower right inset of

*Fig. 5. The conductance G*NS and the normal state
*conduc-tance G*Nare found from Eqs.共3兲and共4兲with the
transmis-sion matrix in Eq.共15兲.

In Fig. 5 we present a calculation of the normalized
*con-ductance g as a function of the normalized barrier strength Z*
*for the device considered by De Raedt et al.*15For the
posi-tion of the Fermi level (䊊*) considered by De Raedt et al.,*
the normalized conductance is only weakly suppressed共
com-pared to a system without a QPC, see, e.g., Ref. 29兲for low
*barrier scattering (Z*⬍1) and only for a very high barrier
*strength (Z*⬎2) the normalized conductance approaches the
*crossover from an excess conductance (g*⬎1) to a deficit
*conductance (g*⬍*1). The effect of the barrier for Z*⬍1 is
very similar to the reflectionless tunneling behavior in
diffu-sively disordered junctions13,17where the net result is as if
tunneling through the barrier is reflectionless. In the case of a
QPC instead of a diffusive region there is a weak dependence
on the barrier strength and the tunneling is not perfectly
re-flectionless.

*An interesting feature is the nonmonotonic behavior of g*
*as a function of Z. For Z→*⬁, the normalized conductance of
course vanishes, but in some regions it increases with an
increasing barrier strength 关curve (䊊)兴*and for Z*⯝1 it has
*the same value as for Z*⫽0. This is purely an effect of size
quantization in the cavity between the QPC and the barrier
which enters the conducting properties because of the fully
coherent propagation of electrons and holes. However,
changing, e.g., the position of the Fermi level slightly
关curves (䉭) and (䊐)兴, changes the quantitative behavior
*although the overall suppression of g with increasing Z is*
maintained.

**C. Incoherent junction**

In junctions where the propagation in the cavity between
the QPC and the NS interface is incoherent, the so-called
*FIG. 4. Normalized conductance g*⬅*G*NS*/G*N of a coherent

*WNW 2DEG-S junction as a function of k*F*W*⬘/. The constriction
*has an aspect ratio L1/W*⬘⫽*5/1.6 and a relative width W/W*⬘
⫽31.72. The curve is based on a numerical calculation of

*t*WNW. The data-point (䊊) corresponds to the numerical
*result (k*F*W*⬘/*;g)*⫽*(3.2;1.87) of De Raedt et al.* 共Ref. 15,
Table I兲.

sequential tunneling regime, the QPC and the NS interface can be considered as two series-connected resistive regions.31 This means that

*G*QPC-NS⫽共*G*QPC⫺

1 _{⫹}

*G*_{NS}⫺1兲⫺1, 共31兲

*G*QPC-N⫽共*G*QPC⫺

1 _{⫹}_{G}

N

⫺1_{兲}⫺1_{,} _{共}_{32}_{兲}

*where G*QPC*and G*Nare found from Eq.共4兲*with t*⫽*t*QPCand

*t*⫽*t*_{␦}*, respectively, and G*NS from Eq. 共3兲 *with t*⫽*t*␦. The
normalized conductance can be written as

*g*⬅*G*QPC-NS
*G*QPC-N ⫽

*G*_{NS}

*G*N⫻

*G*_{QPC}⫹*G*_{N}

*G*QPC⫹*G*NS

, 共33兲

*and for W*Ⰷ*W*

### ⬘

the major contribution to the resistance*comes from the QPC, i.e., G*QPCⰆ

*(G*N

*,G*NS). This means

*that the enhancement of G*

_{NS}

*compared to G*

_{N}has a negli-gible effect on the total conductance so that the normalized

*conductance approaches g*⬃1.

*For an ideal QPC and an ideal interface we have G*QPC

⫽*(2e*2*/h)N,G*NS⫽*(4e*2*/h) M , and G*N⫽*(2e*2*/h) M , where*

*N is the number of modes in the QPC and M is the number of*

modes at the NS interface. The corresponding normalized conductance is shown in Fig. 6.

The sequential tunneling behavior may provide an
expla-nation for the unexpectedly small conductance enhancement
*seen in the experiments of Benistant et al.*18on Ag-Pb
inter-faces with injection of quasiparticles into an Ag crystal
through a point contact. The condition for the electronic
transport to be incoherent is that the distance between the
point contact and the NS interface is longer than the
*corre-lation length Lc*⫽Min(

*l*

in*,L*T),

*l*

inbeing the inelastic
*scat-tering length and LT*the Thouless length.4,6For the ballistic device studied by Benistant

*et al.*

*Lc*⫽

*LT*⫽ប

*v*F

*/k*B

*T*⬃9 m共

*at T*⫽1.2 K) which is much shorter than the dis-tance between the point contact and the NS interface (⬃200 m). Lowering the temperature will increase the

*correlation length and for sufficiently low temperatures (T*

⬃0.05 K) we expect a crossover from the sequential tunnel-ing regime to the phase-coherent regime where the Andreev mediated conductance enhancement should become observ-able.

**VI. DISCUSSION AND CONCLUSION**

For an ideal 2DEG-S interface with a QPC in the normal
*region, the normalized conductance g*⬅*G*NS*/G*N depends
strongly on the position of the Fermi level and only when the
Fermi level corresponds to a conductance plateau a doubling
of the conductance is found. The deviations from the
factor-of-2 enhancement, when the Fermi level does not correspond
to a plateau, can be significant and for a particular example
of the WNW constriction we find that the normalized
*con-ductance can be suppressed to g*⬃1.5 in a system with only
two propagating modes in the constriction. In the presence of
a barrier at the 2DEG-S interface, the normalized
conduc-tance depends strongly on the longitudinal quantization in
the cavity set up by the QPC and the barrier. Depending on
the barrier strength, the length of the cavity and the position
of the Fermi level, this longitudinal quantization may give
rise to both constructive and destructive inferences in the
transmission and thus also in the conductance. Perhaps
sur-prisingly, the effect of the barrier is very much suppressed
共compared to a system without a QPC, see, e.g., Ref. 29兲due
to a very strong back scattering at the return of the
quasipar-ticles to the normal probe. The localization of quasiparquasipar-ticles
in the cavity gives rise to an almost reflectionless tunneling
through the barrier as it is also found in systems with a
diffusive normal region.13,17The interferences due to
local-ization in the cavity will be smeared by a finite temperature
and they are also expected to be suppressed by a finite
in-elastic scattering length compared to the length of the
cavity.32

For the sequential tunneling regime we find that the
con-ductance enhancement vanishes as the number of modes at
the interface becomes much larger than the number of modes
*in the QPC. Our calculations show that the S-matrix *
ap-proach provides a powerful alternative to the time-dependent
*Bogoliubov–de Gennes approach of De Raedt et al.*15in
de-tailed studies of the conducting properties of nanoscale
2DEG-S devices. Even though the back-focusing
phenom-enon of the Andreev reflection is robust against changes in
the geometry,15the electron-hole conversion efficiency itself
is not. Finally, we stress that for a quantitative comparison to
experimental systems, it is crucial to take different Fermi
wave vectors and effective masses of the 2DEG and the
su-perconductor into account.29

**ACKNOWLEDGMENTS**

We would like to thank C.W.J. Beenakker, M. Brand-byge, J.B. Hansen, and H.M. Rønnow for useful discussions. N.A.M. acknowledges financial support by the Nordic Acad-emy for Advanced Study 共NorFA兲 and H.S. acknowledges support by the European Community.

1_{A.F. Andreev, Zh. E}_{´ ksp. Teor. Fiz. 46, 1823}_{共}_{1964}_{兲 关}_{Sov. Phys.}
**JETP 19, 1228**共1964兲兴.

2_{P.G. de Gennes, Superconductivity of Metals and Alloys}_{共}_{}
Ben-jamin, New York, 1966兲.

3** _{C.W.J. Beenakker and H. van Houten, Solid State Phys. 44, 1}**
共1991兲.

4_{Y. Imry, Introduction to Mesoscopic Physics}_{共}_{Oxford University}
Press, Oxford, 1997兲.

5_{T.M. Klapwijk, Physica B 197, 481}_{共}_{1994}_{兲}_{.}

6_{C.W.J. Beenakker, in Mesoscopic Quantum Physics, edited by E.}

Akkermans, G. Montambaux, and J.-L. Pichard共North-Holland,
Amsterdam, 1995兲**; Rev. Mod. Phys. 69, 731**共1997兲.

7** _{C.J. Lambert and R. Raimondi, J. Phys.: Condens. Matter 10, 901}**
共1998兲.

8** _{H. Takayanagi, J.B. Hansen, and J. Nitta, Phys. Rev. Lett. 74, 166}**
共1995兲

*共1995兲*

**; H. Takayanagi, T. Akazaki, and J. Nitta, ibid. 75, 3533****; H. Takayanagi and T. Akazaki, Phys. Rev. B 52, R8633**共1995兲

**; H. Takayanagi, Phys. Rev. B 218, 113**共1996兲; H.

*共1996兲; H. Takayanagi, T. Akazaki,*

**Takayanagi, ibid. 227, 224****and J. Nitta, Surf. Sci. 362, 298**共1996兲; H. Takayanagi, T.

**Aka-zaki, and E. Toyoda, Appl. Supercond. 5, 357**共1997兲.

9** _{C.W.J. Beenakker and H. van Houten, Phys. Rev. Lett. 66, 3056}**
共1991兲.

10** _{H. van Houten and C.W.J. Beenakker, Physica B 175, 187}**
共1991兲.

11_{C.W.J. Beenakker, Phys. Rev. Lett. 67, 3836}_{共}_{1991}_{兲}** _{; 68, 1442}**
共1992兲.

12_{A. Furusaki, H. Takayanagi, and M. Tsukada, Phys. Rev. Lett. 67,}

132共1991兲**; Physica C 185-189, 2585**共1991兲**; Phys. Rev. B 45,**
10 563共1992兲.

13_{C.W.J. Beenakker, Phys. Rev. B 46, 12 841}_{共}_{1992}_{兲}_{.}

14_{Y. Takagaki and H. Takayanagi, Phys. Rev. B 53, 14 530}_{共}_{1996}_{兲}_{.}
15_{H. De Raedt, K. Michielsen, and T.M. Klapwijk, Phys. Rev. B}

**50, 631**共1994兲.

16_{B.J. van Wees, H. van Houten, C.W.J. Beenakker, J.G. }

William-son, L.P. Kouwenhoven, D. van der Marel, and C.T. Foxon,

**Phys. Rev. Lett. 60, 848** 共1988兲; D.A. Wharam, T.J. Thornton,
R. Newbury, M. Pepper, H. Ahmed, J.E.F. Frost, D.G. Hasko,
**D.C. Peacock, D.A. Ritchie, and G.A.C. Jones, J. Phys. C 21,**
L209共1988兲.

17_{B.J. van Wees, P. de Vries, P. Magne´e, and T.M. Klapwijk, Phys.}

**Rev. Lett. 69, 510**共1992兲.

18_{P.A.M. Benistant, A.P. van Gelder, H. van Kempen, and P. }

**Wy-der, Phys. Rev. B 32, 3351**共1985兲.

19_{S. Datta, Electronic Transport in Mesoscopic Systems}_{共}_{}
Cam-bridge University Press, CamCam-bridge, 1995兲.

20

**J. Bardeen, L.N. Cooper, and J.R. Schrieffer, Phys. Rev. 108,**
1175共1957兲.

21_{R. Landauer, IBM J. Res. Dev. 1, 223}_{共}_{1957}_{兲}** _{; Philos. Mag. 21,}**
863 共1970兲

**; D.S. Fisher and P.A. Lee, Phys. Rev. B 23, 6851**共1981兲

**; M. Bu¨ttiker, Phys. Rev. Lett. 57, 1761**共1986兲. 22

_{G.E. Blonder, M. Tinkham, and T.M. Klapwijk, Phys. Rev. B 25,}4515共1982兲.

23_{G.B. Lesovik, A.L. Fauche`re, and G. Blatter, Phys. Rev. B 55,}

3146共1997兲.

24_{G.B. Lesovik and G. Blatter, Pis’ma Zh. Eksp. Teor. Fiz. 68, 572}

共1998兲 关**JETP Lett. 68, 599**共1998兲兴.

25_{A. Szafer and A.D. Stone, Phys. Rev. Lett. 62, 300}_{共}_{1989}_{兲}_{.}
26_{A. Weisshaar, J. Lary, S.M. Goodnick, and V.K. Tripathi, J.}

**Appl. Phys. 70, 355**共1991兲.

27_{F. Kassubek, C.A. Stafford, and H. Grabert, Phys. Rev. B 59,}

7560共1999兲.

28_{M. Kupka, Physica C 281, 91}_{共}_{1997}_{兲}_{.}

29_{N.A. Mortensen, K. Flensberg, and A.-P. Jauho, Phys. Rev. B 59,}

10 176共1999兲.

30_{F.A. Maaø, I.V. Zozulenko, and E.H. Hauge, Phys. Rev. B 50, 17}

320共1994兲.

31_{M. Bu¨ttiker, Phys. Rev. B 33, 3020}_{共}_{1986}_{兲}** _{; IBM J. Res. Dev. 32,}**
72共1988兲.

32_{For a recent approach including possible interactions, see, e.g., Q.}